effect of twist on the physical properties of a number 7s yarn
Post on 15-Dec-2016
Embed Size (px)
EFFECT OF TWIST ON THE PHYSICAL PROPERTIESOF A NUMBER 7S YARN
By F. R. McGowan, Charles W. Schoflstall, and A. A. Mercier
This investigation was made to determine the most suitable twist for manu-facturing the yarn to be used in the Pima post office bag investigation. Datawere obtained on the relation of the twist to the breaking strength, diameter
of the yarn, yarn count, contraction, and angle of twist. While these data
were not sufficiently extensive to attempt to fix definite formula for these
relations, it is thought that the tabular and graphical relation studied in thisinvestigation will be useful for the cotton manufacturer. The most suitabletwist for the yarn to be used in the Pima mail bags was found to be about 12turns per inch.
I. Introduction 85
II. Purpose 86
III. Method of manufacture 86
IV. Methods of test 87
1. Contraction 87
2. Yarn count 87
3. Diameter of yarn .. 87
4. Angle of twist 88
5. Breaking strength 89
V. Discussion of results 89
VI. Summary 95
There are many different ideas regarding the amount of twist 1
which should be given to a cotton yarn to serve any specific purpose.
These opinions have been founded more or less on observation andfact, but sometimes they have no sound reasonable basis. For in-stance, the terms " hosiery twist," " warp twist," " filling twist,"etc., are used with numerous ideas as to just what they comprise,
for they vary considerably from mill to mill, and even within theorganization of a single mill marked variations in practice occur.This condition results primarily on account of lack of fundamental
data. If it were known, for example, just what is the effect of achange in the twist on the breaking strength, diameter, etc., of the
yarn, a more comprehensive basis for fixing the organization require-ments in the manufacture of the yarn might be obtained.
1 The twist of the yarn may he defined as the number of turns in a definite length ofyarn, as turns per inch.
86 Technologic Papers of the Bureato of Standards [vol. 19
Data available on the effect of a change in twist on the otherphysical properties of the yarn should be very useful to the cotton
manufacturer. The data on the effect on the diameter alone willsolve many difficulties, for a change in diameter may necessitate achange in threads per inch. In that case unless the threads per inch
were changed there would result a definite change in the appear-
ance and probably the usefulness of the fabric. The effect of achange of twist on the breaking strength is of vital interest to manu-facturers of those mechanical fabrics, the strength of which is an
influencing factor. While the effect of a change in the angle of
twist is not so directly evident, various uses may be found forthese data.
It is with this idea that the results of this investigation are offered
with the hope that it will be useful as a basis for further work alongthis line. The immediate need for these data at this bureau was tofind the most suitable twist for the manufacture of yarns to makeduck for the use of post-office mail bags.2
The purpose of this investigation was to determine the effects onthe physical properties of the yarn, resulting from changing the
twist in the spinning process on number 7s cotton yarn. Thephysical properties studied were yarn count, diameter, contraction,angle of twist, and breaking strength.
III. METHOD OF MANUFACTUREThe cotton used in this investigation was classed as No. 2 Pima,
or Arizona-Egyptian cotton, fully equal to middling Upland ingrade. The average staple length was 1% inches.The number of mill processes were kept as few as possible and
still produce a good quality of yarn.
The following organization was used : 3
Vertical opener [l4.4-ounce lap.
Breaker picker ]
Finisher picker 11.6-ounce lap.
Card 45-grain sliver.
Drawing frame 1Drawing frame > 46-grain sliver.Drawing frame J
Slubber 1.04-hank roving.
Spinning frame 7s yarn.
2 Comparative Wearing Qualities of Pima and Ordinary Cotton Used in Mail Bags, B. S,Tech. Taper No. 277.
3 Complete organization is given in B. S. Tech. Paper No. 277.
schJffstaii] Effect of Twist on Pima Yarn 87Meroier J
When the fibers are delivered from the front roll of the spin-ning frame they are practically parallel, but they are twisted im-
mediately to an extent which will give them sufficient strength sothat the yarn can be wound on the bobbin in a continuous strandand can proceed through the further processes of manufacture
without breaking. While the lowest limit of twist is generally de-termined by the workability of the yarn, the number of turns ad-ditional in the later processes depended upon the use for which the
yarn is intended.
In this investigation the twist was varied at the spinning frameto produce from about 7 to 19 turns per inch. The same draft(ratio of input to output) was used for all twists.
IV. METHODS OF TESTi. CONTRACTION
Contraction in the yarns is the decrease in their length produced
by some physical or chemical force. This can be caused, as was the
case in this study, by an increase in the twist. A measure of thecontraction can be obtained in two ways
(a) Weight Determination.The difference in weight for agiven number of yards before and after the twisting process; thatis, weight difference divided by length.
(&) Draet Measurements.^As the yarn contracts with increasein twists, it is necessary to regulate the draft in order to keep the
weight of the yarn constant. The feed is, therefore, diminished inproportion to the increase in weight. This amount can be calcu-
lated and the contraction ascertained.
In this investigation, since the same draft was used for all twists,
the contraction was measured from the increase in weight only. Themethod used was as follows: After conditioning for at least fourhours in an atmosphere of 65 per cent relative humidity and 70 F.
temperature, from each of three bobbins of each different twist ahank of 120 yards was reeled and weighed.
2. YARN COUNT
The yarn size is figured on the basis of the number of yards fora definite weight. In the case of cotton it is the number of 840-yardhanks which will weigh 1 pound. The results in this investigationwere obtained from the weights of 120-yard lengths above men-tioned.
3. DIAMETER OF YARN
The diameter of the yarn of a definite weight varies as the twistis increased or decreased. The low-twisted yarn is larger in
88 Technologic Papers of the Bureau of Standards [Val. 19
diameter and softer than the hard-twisted yarn. The procedureused to measure the diameter of the yarn was as follows: A photo-graph of several lengths of yarn which had been magnified 40times was taken. On these prints, several of which are shown inFigure 1, at intervals of 1 inch a measurement of the diameter wasmade in one-sixteenth inch.
4 . ANGLE OF TWIST
Attention has already been called to the reasons for twisting the
yarn. The angle of the twist resulting from the twisting opera-
Technologic Papers of the Bureau of Standards, Vol. 19
Effect of Twist on Pima Yarn
5. BREAKING STRENGTH
The twist is an important factor in obtaining the strength of ayarn. In the twisting process the fibers are entwined around andcling to each other, so that they resist efforts to slip by each other.
Theoretically the maximum strength is obtained when sufficienttwist is given which will, with minimum strain to the individualfibers, prevent any slipping when force is applied in a longitudinaldirection. Beyond this point the strength decreases and this de-crease can be continued until the yarn breaks under no longitudinal
strain, but merely from the shearing action of the twisting. Bursts
occurring from excessive twist are evident in Figure 1. Excessive
twisting, in addition to lowering the breaking strength, causes kink-
ing in the yarn, which renders it difficult to handle.
The strength of the yarn is not always the governing factor in
preparing a textile material for use. It has been pointed out that
the greater the twist the harder the yarn. This hardness may be anundesirable quality, and it may be necessary to sacrifice the strengthfeature to obtain a characteristic which is more desirable for the use
for which the product is intended. Knitting yarns, for instance, are
generally soft, low-twisted yarns, because the yarns are easier to
handle on the knitting process, and the resulting product is desired
to be of soft quality.
The breaking-strength method used was the single-end method.For each strength determination three bobbins of yarn were taken
at random, from each of the various lots of different twists. All
tests were made after conditioning for at least four hours in anatmosphere of 65 per cent relative humidity and 70 F. temperature.The testing was done on an inclination balance type of machine.Ten to twenty breaks were made from each bobbin, and these breakswere averaged for the bobbin, and then these averages were averagedto obtain the result for that particular twist.
V. DISCUSSION OF RESULTS
A summary of the tests are given in Table 1.Table 1.
Summary of results on Pima, yarn (7s) of varying ticists
DiameterA inch,magnifi-cation .40X